atw Vol. 63 (2018) | Issue 3 ı March
60 mm while the diameter of the inner
fuel containing matrix is 50 mm .
Figure 11 shows the difference
between the first idea of a pebble with
non-coated fuel and the current type.
The inner diameter of the coated fuel
particles is 0.5 mm. Embedded in the
inner graphite matrix are approximately
15,000 coated particles (cp) in
one pebble and contain the fuel
material (Figure 12). The fuel kernel
is encapsulated by three layers of very
hard and pressure resistant PyC-/-SiC-
/-PyC and is gas tight (Figure 13).
These are the “TRISO” Fuel Elements
and each coated particle has a
diameter of 0.9 mm.
| | Fig. 14.
Treatment of pebbes by hand, first pebble
loading into the core of the AVR-HTR.
| | Fig. 15.
Storage of burnt-down pebbles in casks.
describes results of an experiment: “A
High Voltage Head-End Process for
Waste Minimization and Reprocessing
of Coated Particle Fuel for High
Temperature Reactors.”  This
process is proposed for the separation
of coated kernels from the fuel matrix
and makes it possible to reprocess the
burnt down fuel by separation of the
coatings and the fuel kernel. The fuel
kernels remain intact and has been
successfully demonstrated in experiments
as shown in Figure 16, 17, and
18. The characteristics of the coated
fuel kernels and the complete pebbles,
manufactured by NUKEM, is shown in
This process, proposed and studied
with experiments by EU-JRC-Petten,
envisages the complete removal of the
coating-layers to make the fuel accessible
for further reprocessing and
manufacturing of new fuel kernels.
RESEARCH AND INNOVATION 171
| | Fig. 13.
Composition of a TRISO-pebble.
Without coating the radioactivity
of the primary helium gas in the AVR
was calculated initially to be 10 7
Curie. Therefore, the AVR was
designed with two pressure vessels.
All piping and helium operated components
were surrounded with clean
helium gas, to prevent primary contaminated
Helium gas from entering
the reactor vessel. These fuel elements
were not initially used.
The newly developed TRISO
elements avoid fission and decay
products, which are the sources of
dangerous radioactivity. Three layers
form a containment for every CP
and keep all fission products safely
enclosed. The layers remain gas tight
from 1,620 °C to 1,800 °C and do not
deteriorate or corrode even under
As previously mentioned, AVR
was initially designed with a helium
primary gas activity of 10 7 Curie. After
the development of the pebbles with
coated particles the primary helium
gas activity was measured at only
360 Curie , a factor of 0.000036
lower. They were proven in long term
operation in the AVR as reliable fuel
elements and have very excellent
advantages in comparison with all
fuel elements in other nuclear power
Fresh pebbles can be stored and
handled without any risk of radiation
(Figure 14). Radiated, burnt down
pebbles or graphite balls will be stored
(Figure 15). primarily in specially
designed containers or stockrooms
inside the basement of the reactor
building. No cooling is necessary and
they can be stored over a longtime
without risk of contamination or
radiation of the surrounding area or
personnel [15, 16, 17].
Breeding of fissile Uranium-233
by using Thorium-232
Sufficient Thorium can be found in
the surface of the earth to generate
electricity and heat by nuclear power
stations for a very long time. [20, 21,
22] However, fissile fuel needs to be
produced from the Thorium. This is
possible by breeding 232 Th up to 233 Th
using slow neutrons initially resulting
in Protactinium ( 233 Pa) which decays
to fissionable 233 Uranium. This process
is a very good possibility in a
THTR power station.
The coated fuel kernels can contain
Uranium 235/238, Plutonium 238-
242, or Thorium 232 [15, 17, 18].
These fuel materials can be combined
in a pebble matrix and burned
together. After extracting the core,
every single pebble can be measured
to its degree of burn-up. In HTR-
Pebble Bed reactors the disposal of Pu
can be extensively controlled and
each pebble is treated individually. A
very detailed and full control of Pu
disposal is guaranteed and possible
through inspection to meet the NPT.
Decommissioning and Reprocessing
of Fuel Elements and
The paper by the Netherlands
European Joint Research Centre JRC
Pebble Bed Ring-Core Design
for very large TVHT-Reactors
Important discoveries were generated
from the long-term operation of
the AVR and relatively short period
of three years operation of the
THTR-300, The information obtained
from these two power plants is
Particle batch HT 354-383
Kernel composition UO 2
Kernel diameter in
[U-235 wt. %]
Thickness of coatings
Inner PyC 38
Outer PyC 41
Particle diameter 909
Heavy metal loading
Number of coated
particles per pebble
Defective SiC layers
[U/U tot ]
7.8 x 10 -6
Matrix graphite grade A3-3
Matrix density [kg/m 3 ] 1,750
Temp. at final heat
| | Tab. 2.
Typical chracteristics of coated particles and
pebbles produced by NUKEM.
Research and Innovation
The Technology of TVHTR-Nuclear- Power Stations With Pebble Fuel Elements ı Urban Cleve